00 PLASTICIZED ETHYLENE -V'!NYL ACETATE Mw BINDERS FOR INSENSITIVE BOOSTER _-. COMPOSITIONS W I.J. DAGLEY. R.P. PARKER. L. MONTELLI AND C.N. LOUEY MRL-TR-91-34 DTIC SI ELECTEI FEB6 This document has been apptoved for public release and sale; its distribution is unlimited. APPROVED FOR PUBLIC RELEASF .QTr;
00 PLASTICIZED ETHYLENE -V'!NYL ACETATEMw BINDERS FOR INSENSITIVE BOOSTER
W I.J. DAGLEY. R.P. PARKER. L. MONTELLI AND C.N. LOUEY
This document has been apptovedfor public release and sale; itsdistribution is unlimited.
FOR PUBLIC RELEASF
Plasticized Ethylene-Vinyl AcetateBinders for Insensitive Booster
.1. Dagley, R.P. Parker, L. Montelliand C.N. Louey
MRL Technical ReportMRL-TR-91-34
Plasticizers have been incorporated into RDX/ethylene-vinyl acetate (EVA)compositions prepared by the solvent slurry coating technique. The effect ofplasticizers on impact sensitiveness, shock sensitivity, cookoff behaviour and integrity ofpressed pellets has been examined for compositions with EVA binders of varying vinylacetate content. A compatible EVA/plasticizer combination gave an appreciablereduction in cookoff response and impact sensitiveness. Plasticizer migration is likelyto affect the long-term stability of these compositions.
NTIS CRA&IDTIC TAB Li
Commonweelth of Australia Justification
B y ........... . ... ............... .
..... . . ,i , . _ D i t ib io.:
Avod a. d_Dist Is -
frMATERIALS RESEARCH LABORATORY -
9 2 2 210 03 5 3Iiih1 |I1 i
Materials Research LaboratoryCordite Avenue, MaribyrnongVictoria, 3032 Australia
Telephone: (03) 319 3887Fax: (03) 318 4536
Q Commonwealth of Australia 1991AR No. 006-827
APPROVED FOR PUBLIC RELEASE
Dr Ian Dagley attended University of Melbourne,graduating BSc (Hons) in Chemistry and PhD inOrganic Chemistry in 1979. He was awarded a PerkinFellowship for two years postdoctoral studies at OxfordUniversity, then returned to Australia in 1981 to beChief Chemist at Beta Chemical (Dunlop-Olympic). Ianjoined Explosives Division, MRL in 1985, where he hasconducted R & D on booster explosives, insensitive highexplosives, and mechanisms of their initiation undermechanical impact.
Robert Parker graduated Dip App Chem from BallaratSchool of Mines and Industries in 1968, and joined MRLin that year. He has worked exclusively on explosivemateriaLs; his present major areas of interest aie cookoffof explosives and PBX formulations.
Lucianna Montelli graduated BAppSc in Chemistry in1987 from Royal Melbourne Institute of Technology.She was then recruited to MRL where she has conductedR & D into a number of aspects of explosives technologyincluding polymer bonded explosives formulation andthermally stable high explosives for initiating devices.
Craig Louey graduated BApplSc (Hons) in Chemistry in1987 from University of Melbourne. He was recruitedto MRL in 1988 where he worked exclusively in theExplosives Materials area, specialising in desensitisationof explosives through the use of polymers. Craig hasnow left MRL.
3.4.1 Rotter Impact Sensitiveness: Figure of Insensitiveness (F of 1) 103.4.2 Shock Sensitivity: Small Scale Gap Test 103.4.3 Cookoff Test 11
4. RESULTS AND DISCUSSION 124.1 Impact Sensitiveness and Shock Sensitivity 124.2 Pellet Integrity and Plasticizer Migration 1443 Cookoff Behaviour 14
5. CONCLUSIONS 16
6. ACKNOWLEDGEMENTS 17
7. REFERENCES 17
Plasticized Ethylene-Vinyl AcetateBinders for Insensitive Booster
For decades Australian ordnance has typically contained tetryl as the fuzebooster composition and TNT-based main charge fillings. These compositionsare vulnerable to unplanned hazardous stimuli (e.g. bullet/fragment impact,fuel fire, detonation of adjacent charges) and must be replaced in newAustralian ordnance currently being designed to meet insensitive munitionscriteria. Less sensitive polymer bonded explosive (PBX) compositionsdeveloped overseas are being evaluated at MRL as alternative main chargecompositions . Because overseas technology for insensitive boostercompositions was less advanced, a project to develop a suitable pressedcomposition for use in Australian production and filling was commenced atMRL.
Ideally the new booster composition should:- be no more sensitive than tetryl to initiation by impact for compliance
with current fuze explosive train guidelines [21,- be no more sensitive than tetryl to shock initiation,- have pickup and output properties similar to those of tetryl,- respond mildly (deflagration or less) under both fast and slow cookoff
conditions, and- be processible on a small batch scale in existing or easily acquired plant.
Insensitive PBX booster compositions developed in the US and UK containnitrarnines (RDX or HMX), to confer shock sensitivity and performance, inblends with more thermally stable and less sensitive high explosives(e.g. TATB) [3, 41. Most overseas research has concentrated on optimizingthese blends to achieve the desired level of sensitivity and vulnerability.. Incontrast the early stages of the Australian study have focused more closely onbinder selection and coating techniques since sensitivity and vulnerability are
also influenced by the properties of the binder and the extent to which it coatsthe explosive crystals [5, 61. By adoping this approach it should be possible toplace less reliance on blending explosives to obtain the correct balance ofproperties.
Initial studies examined the sensitivity and cookoff response of numerousRDX/polymer (95:5) compositions prepared by the slurry and dispersioncoating processes [7, 81. Certain ethylene-vinyl acetate (EVA) copolymersmoderated the sensitivity and vulnerability of RDX. The properties of EVAcopolymers are largely determined by their vinyl acetate content (quoted asweight percent (% VA) in this report) and their molecular weight. The effectsof variations in these parameters on the impact sensitivity and shock sensitivityof these compositions have been largely explained [5, 71; in contrast norelationship has been established between the structure or properties of thesecopolymer resins and their ability to moderate cookoff response. In this caseminor differences in properties produced marked effects on cookoff responsebut the experimental data did not reveal any obvious correlations.
In an extension of this project, the possibility of achieving further reductionsin sensitivity and vulnerability of RDX-based compositions by modifying theproperties of their EVA binders with low levels of plasticizers has beeninvestigated. This study has focused largely on modifying one EVA binder,Levapren 408, which contains 40% VA and has a comparatively low molecularweight. This copolymer was typical of the majority of EVA resins examined inan earlier study - it did not reduce the impact sensitiveness of RDX orsignificantly modify its cookoff response. A copolymer containing a lowervinyl acetate content (28% VA) with a low molecular weight (Elvax 210) andone containing a higher vinyl acetate content (50% VA) with a high molecularweight (Levapren 500) were markedly better than other EVA copolymers atmoderating fast cookoff response. Both these copolymers were also plasticized,primarily to achieve further moderation of cookoff response.
2. Experimental Approach
RDX/Levapren 408/plasticizer (95:5:0.5) moulding powders containing a rangeof plasticizers were prepared and their impact sensitiveness was assessed. Theshock sensitivity of compacts prepared from promising compositions containingphthalate, flame retardant and polymer plasticizers was then determined. Theplasticizer from each class that gave the least shock sensitive compact was usedto prepare compositions containing the EVA copolymer with lower vinyl acetatecontent (Elvax 210). The impact sensitiveness of these compositions wasdetermined and their cookoff response was compared to that of the equivalentcompositions containing Levapren 408 and, in one case, Levapren 500.
RDX Grade A, Class 1 (recrystallized) from Albion Explosives Factory was usedto prepare all compositions. It was received wet and thoroughly dried at thepump prior to use.
The EVA copolymers examined were Levapren 408 and Levapren 500 fromBayer and Elvax 210 from Du Pont; they have vinyl acetate contents of 40, 50and 28 percent respectively.
The plasticizers used in these experiments and their commercialmanufacturers are listed in Table 1. All the solvents used were laboratorygrade. Distilled water was used in all the preparations. Mowiol 4-88 is apartially saponified polyvinyl alcohol manufactured by Hoechst and was usedas a protective colloid to stabilize the emulsion formed between the polymersolution and water during the slurry coating process.
Table 1: Chemical Descriptions and Manufacturers of Plasticizers Used inCompositions
Material Chemical Description Manufacturer
Adipate and Phthalate Plasticizers
DOA Dioctyl adipate CSR Chemicals
DOP Dioctyl phthalate CSR Chemicals
Edenol DCHP Dicyclohexyl phthalate Henkel
Flame Retardant Plasticizers
Fyrol FR-2 Tris(,p'-dichloro-isopropyl) Stauffer Chemicalphosphate Company
Re-plas 1360 High molecular weight long Townsend Chemicalschain polyester
Repol 720 Linear polyester diol (molecular Townsend Chemicalsweight 2200)
3.2 Mixing Equipment
Batches of these compositions were prepared in an open metal mixing vesselfitted with a heating jacket and containing two internal baffles mountedperpendicular to the walls of the vessel. The slurries were stirred by anoverhead air motor driving a rod with an impeller at the base equipped withtwelve flat blades.
3.3 Preparation of RDX/EVAPlasticizer (95: 5: 0.5)Compositions
A slurry of RDX (142.5 g) and water (430 mL) was stirred at 500 r/rin for5 min then an aqueous solution of Mowiol 4-88 (0.01% w/w, 15 mL) was addedand the slurry was heated to 65°C. After a further 10 min a solution of theEVA copolymer in toluene (10% w/w, 75 g) containing the dissolved plasticizer(0.75 g) was slowly added. The mixture was stirred vigorously at 700 r/minand the temperature of the slurry was maintained at 65°C until the solvent hadevaporated and hard moulding granules had formed. The agitated slurry wascooled to 30PC and the collected granules were washed with water, dried at thepump and then at 60C ander vacuum over silica gel.
3.4.1 Rotter Impact Sensitiveness: Figure of Insensitiveness (F of I)
A Rotter apparatus  fitted with a 5 kg weight was used to determine theimpact sensitiveness of the compositions. The results were obtained using25 caps and the tests were carried out in accordance with the Brucetonprocedure. The F of I values quoted, derived from the height for 50% initiationprobability, are relative to RDX Grade F = 80 and are rounded to the nearestfive units. The average gas volumes for positive results are also quoted.
3.4.2 Shock Sensitivity : Small Scale Gap Test
The MRL small scale gap test (SSGT) 1101 was used to obtain the shocksensitivity data. A UK Mk 3 exploding bridge wire detonator was used as thedonor and the shock was attenuated by brass shim. The acceptor was two12.7 mm diameter x 12.7 mm high cold pressed cylinders of the explosiveunder study. A detonation was confirmed using a mild steel witness block.The results were obtained from 20 to 30 firings using the Bruceton staircasemethod and are quoted in mm of brass shim for a 50% detonation probability,together with the 95% confidence limits and standard deviation.
3.4.3 Cookoff Test
The cookoff behaviour of the compositions was assessed using the Super Small-scale Cookoff Bomb (SSCB) [111. Samples were pressed at 90% TMD(theoretical maximum density) into pellets 16 mm diameter x 16 mm long, andfour pellets were used per test. Tests were performed at fast (approximatelyPC/second) and slow (approximately 0.1 0C/second) heating rates. ModifiedSSCBs were used for some of the tests. The original and modified SSCBs areshown in Figures la and lb respectively. The major differences are theelimination of the large air space and the closing plug from the top of the testassembly (giving a symmetrical geometry) and the use of a single full-lengthinner cylinder instead of two half-length cylinders. Results from a number oftests indicate that the modifications do not affect the rating of the type ofresponse obtained or the temperature at which reaction occurs, however theheating rates obtained with the modified SSCB are slightly lower than with theoriginal test assembly [121.
r" r Top plate Washer
---- Outer cylinder a- n
Figure 1: (a) Original SSCB and (b) Modified SSCB.
4. Results and Discussion
4.1 Impact Sensitiveness and Shock Sensitivity
The impact sensitiveness data for the various RDX/Levapren 408/plasticizer(95:5.-0.5) moulding powders is listed in Table 2. All the compositions, exceptthe one containing Re-plas 1360, were significantly less sensitive to impact(F of I values of 90 to 105) than the moulding powder without plasticizer(RDX/Levapren 408 95:5, F of I = 75). Two factors that lead to a reduction inimpact sensitiveness of RDX/EVA moulding powders are an improvement inthe way the binder coats the explosive crystals and greater flow by the polymerduring impact. In the latter case greater flow allows the polymer to moreefficiently quench hot spots and, as a result of a reduction in viscosity, notundergo heating to such high temperatures . Either or both of these factorsmay be contributing to the reduced impact sensitiveness of these plasticizedmoulding powders. Granular tetryl has an F of I of 90 [131, and this figure isthe accepted limit for acceptability of materials below the shutter in afuze train .
Table 2: Impact Sensitiveness of Various RDX/EVA/Plasticizer (95:5.D.5)Compositions
EVA Polymer and Plasticizer F of I& Gas Evolution (mL)
a Relative to RDX Grade F = 80. b Data from reference 7.c Data from reference 13. d Data from reference 14.
Typical production batches of both granular and crystalline tetryl have F of Ivalues of 105 to 110 [141. Most of the plasticized RDX/Levapren 408compositions have F of I values within the range of those of tetryl and wouldbe acceptable compositions in this respect.
Some RDX/Levapren 408 compositions containing different phthalate andpolymeric plasticizers and one flame retardant plasticizer (see Table 1) werepressed to 90% TMD and their shock sensitivity was determined; results arepresented in Table 3. All these compositions were less shock sensitive thanRDX (250 to 300 pm) and granular tetryl, and more shock sensitive than theunplasticized RDX/Levapren 408 and PBXW-7 Type II (an insensitive boostercomposition developed in the US). The shock sensitivity of pressed RDX/EVAmoulding powders has been examined and the nature of the voids in thecompact (determined by the binder plasticity), relative coating efficiencies of thepolymers on the surface of the crystals in the moulding powders, the highstrain-rate mechanical properties of the pressed pellet and susceptibility forcracking under shock loading may all influence sensitivity in this test . Therelative shock sensitivities of the pressed plasticized compositions may also beinfluenced by the extent of plasticizer migration in the pressed pellet whichmay have occurred between pressing and testing these compositions (seesection 4.2).
Table 3: Shock Sensitivity (SSGT) of RDX/Levapren 408/Plasticizer (95:5:0.5)Compositions
Plasticizer Relative Density Shock Sensitivity (mm)'(% TMD) M5o% Range Lg% Standard Deviation
RDX, Grade A (250- 90.00 3.360 3.622-3.100 0.12300 Prm sieve cut) ITetryl, granular d 90.0 3.259 3.315-3.203 0.021PBXW-7 Type 1I d 90.0 1.415 1.448-1.382 0.015
a All figures are in mm of brass shim. b Data from reference 7.c Data from reference 15. d Data from reference 16.
The phthalate, polymeric and flame retardant plasticizers (Edenol DCHP,Repol 720, Reofos 65) that gave the least shock sensitive compositions wereused to prepare RDX/EVA/plasticizer 95:5:0.5 compositions containing an EVAresin with a lower vinyl acetate content, Elvax 210, for comparative cookoffstudies. The impact sensitiveness of these moulding powders was also
measured (see Table 2). The compositions were as sensitive or more sensitiveto impact than the moulding powder without plasticizer (RDX/Elvax 210, 95:5,F of I = 90 to 130).
4.2 Pellet Integrity and Plasticizer Migration
The pressed pellets prepared for cookoff testing were stored for several monthsunder ambient conditions prior to use. It was found that the pellets ofRDX/Elvax 210 with Edenol DCHP and Reofos 65 plasticizers became crumblyon storage, and the surfaces roughened and became dull; in some cases slighttackiness was noticed at the lower end of the pellet. These pellets also "grew"appreciably on storage, from the original diameter of 15.9 mm to about16.1 mm. The pellets of RDX/Levapren 408 with Edenol DCHP and Reofos 65plasticizers aged better, retaining their smooth finish and showing little or notendency to crumble or chip at the edges. They also grew less, havingdiameters of 15.95 to 16.00 mm when tested. The RDX/Levapren 500/Reofos 65pellets were also noted as being smooth and non-crumbly, and had diametersless than 16.00 mm; however they were not stored for as long as the otherpellets, being used within a few weeks of pressing. Pellets of RDX/Elvax 210/Repol 720 and RDX/Levapren 408/Repol 720 aged well, showing only slightroughening of the end faces and maintaining their diameters between 15.95 and16.00 mm. The RDX/Levapren 408/Repol 720 pellets were slightly crumbly atthe edges.
Pressed pellets of all the plasticized compositions, both for shock sensitivityand cookoff tests, were found to produce "grease spots" under the pellets in thecardboard containers in which they were stored, even after relatively shortperiods at ambient conditions. This is considered to be due to migration ofplasticizer from the pellets. The tackiness noticed with some of theRDX/Elvax 210/plasticizer SSCB pellets is believed to be due to the samereason. For the limited range of plasticizers used with different EVA binders,this migration problem appeared to be more severe with the binder with thelower vinyl acetate content (Elvax 210, 28% VA) than with binders with highervinyl acetate contents (Levapren 408, 40% VA and Levapren 500, 50% VA).This is probably due to differences in physical compatibility between theplasticizers and the various EVAs; it is recognized that compatibility ofpolymer/plasticizer combinations is dependent upon the chemical structures ofboth materials . Experiments to quantify the extent of plasticizer migrationhave not been undertaken.
4.3 Cookoff Behaviour
The results of SSCB tests on plasticized RDX/EVA compositions are shown inTable 4, together with previously reported results for the equivalentunplasticized compositions .
Table 4: Cookoff Test (SSCB) Results for Plasticized RDX/EVA Compositions
Composition Heating Temperature Time ResponseRate (OC) (s)
RDX/Levapren 500/Reofos 65 Fast 241 293 Deflagration
955:05 Slow 221 1852 Explosion
RDX/Levapren 5 0 0 b Fast 274 293 Deflagration c
955 Fast 240 255 Deflagration C
Slow 217 1704 Detonation
Slow 217 1592 Mild explosion"A
a. Traces of explosive on parts after test.b. Data from reference 7.c. Appreciable amounts (> 2 g) of unconsumed explosive recovered after test.
d. Composition prepared by alternative (confidential) method.
The RDX/Elvax 210/plasticizer compositions all showed more violentresponses than the unplasticized composition when tested at the fast heatingrate; all three plasticized compositions gave responses as severe as detonations,in marked contrast to the unplasticized composition which gave no reactionmore severe than a mild explosion. The plasticized compositions all showedslight reduction in the response violence at the slow heating rate, in two cases(Edenol DCHP and Reofos 65) giving detonation and explosion responses, andin one case (Repol 720) giving deflagration and explosion responses.
RDX/Levapren 408 exhibits violent cookoff behaviour. Incorporation ofEdenol DCHP plasticizer had little effect on the type of response - detonationswere obtained at both heating rates, although in one test an explosion wasobtained at the fast heating rate. Repol 720 plasticizer gave slight reductions incookoff violence, with explosions being observed at both fast and slow heatingrates, although one test at the fast heating rate gave a detonation. Reofos 65plasticizer, however, had a pronounced effect, giving responses of burn andmild explosion at the fast heating rate, and explosions at the slow heating rate.The effect of this plasticizer on RDX/Levapren 408 is in marked contrast to itseffect on RDX/Elvax 210 (see above); this difference may be due to improvedcompatibility between this plasticizer and the binder with a higher vinyl acetatecontent (40% VA for Levapren 408 cf. 28% VA for Elvax 210).RDX/Levapren 500 exhibits milder cookoff responses than RDX/Levapren 408but also has a high vinyl acetate content binder (50% VA); however, theaddition of Reofos 65 to this composition did not result in a similar reduction ofresponse violence - the plasticized and unplasticized compositions behavedsimilarly. The different effects of plasticizers on the cookoff response of thevarious RDX/EVA compositions is the subject of further research at thislaboratory.
Plasticizers can be incorporated into RDX/EVA binder compositions preparedby the solvent slurry coating technique. Pressed pellets of the plasticizedcompositions were found to vary in their mechanical integrity after storageunder ambient conditions, and evidence of plasticizer migration from thepressed pellets was observed for all compositions. These effects are believed tobe due to the physical compatibility of the EVAs and the plasticizers, and varywith plasticizer composition and vinyl acetate content of the EVA. EVAs withhigher vinyl acetate contents appeared to be more compatible with theplasticizers examined.
Incorporation of a range of plasticizers into RDX/Levapren 408 generally ledto a decrease in impact sensitiveness and a slight increase in shock sensitivity.With RDX/Elvax 210 (with a lower vinyl acetate content EVA), theincorporation of plasticizers generally led to increased impact sensitiveness.RDX/Levapren 408/Reofos 65 (a flame retardant plasticizer) showed asubstantial reduction in the violence of the cookoff response; however, thissame plasticizer had little effect on the cookoff response of RDX/Levapren 500,and led to more violent responses with RDX/Elvax 210. Other plasticizers also
increased the cookoff violence of RDX/Elvax 210 at a fast heating rate, althoughsome moderation was obtained at a slower rate.
Overall, it appears that compatible EVA/plasticizer combinations can giveappreciable reductions in cookoff response and impact sensitiveness of RDX-based booster compositions, but less compatible EVA/plasticizer combinationswill have the opposite effect.
Plasticizer migration, observed with all compositions under laboratoryambient conditions within several months, indicates that long-term stability ofthe compositions under service conditions would be a major problem.Accordingly, development of plasticized booster compositions will not bepursued further. However, a compatible binder/plasticizer combination maybe a possible future option if other current approaches to development of aninsensitive booster composition (e.g. use of other explosives, particle sizemodification) prove to be unsuccessful.
Considerable technical assistance was provided by Mrs B. Pletikapa (cookofftesting), Mr E. Wanat (Rotter testing), Mrs J. Pinson (Rotter testing and vacuumthermal stability testing), Mr J. Pisani (vacuum thermal stability testing),Mr M.G. Wolfson (SSGT) and Mr T. Ryan (SSGT).
Dr R.J. Spear has assisted this project through several useful discussions.The contribution of all these people is gratefully acknowledged.
1. Spear, R.J. (1990).Australian R & D on insensitive munitions. Addendum Proceedings of JointGovernment/Industry Symposium on Insensitive Munitions Technology, WhiteOak, MD, USA, p. 197.
2. (a) US Department of Defense (1984). Military standard. Fuze, designsafety, criteria for, MIL-STD-1316C.(b) UK Ordnance Board (1983). Safety of fuzing systems, OB Proc. 42240.(c) North Atlantic freaty Organization ( ). Fuzing systems - Designsafety requirements, STANAG 4187.(d) Australian Ordnance Council (1990). Principles and criteria for theassessment of explosives initiation systems for safety and suitability for service.AOC Proceeding 174.90.
3. Baudler, B. and Montesi, L.J. (1986).Qualification test results of PBXW-7 Mod I (NSWC/TR-86-22).White Oak, MD: Naval Surface Warfare Center.
4. Hutchinson, C.D. (1985).Experimental studies concerning the response of intermediate explosivesto thermal stimuli. 8th Symposium (International) on Detonation,Albuquerque, NM, USA, p. 1105.
5. Dagley, I.J. and Ho, S.Y. (1991).Impact sensitiveness of RDX with ethylene-vinyl acetate (EVA)copolymers. ICT Internationale Jahrestagung, Karlsruhe, Germany, p. 92.
6. Anderson, C.M. and Pakulak, Jr., J.M. (1977/78).Journal of Hazardous Materials, 2, 143.
7. Dagley, I.J., Spencer, H.J., Louey, C.N. and Parker, R.P. (1989).An examination of ethylene-vinyl acetate copolymers on desensitizers for RDX ininsensitive boosters prepared by the slurry coating technique (MRL TechnicaReport MRL-TR-89-33). Maribyrnong, Vic.: Materials ResearchLaboratory.
8. Dagley, I.J., Montelli, L., Parker, R.P. and Louey, C.N. (1989).Preparation, characterization and cookoff behaviour of booster compositionsprepared from RDX and acrylic or ethylene-vinyl acetate dispersions (MRLTechnical Report MRL-TR-89-44). Maribyrnong, Vic.: Materials ResearchLaboratory.
9. (a) Mortlock, H.N. and Wilby, J. (1966).The Rotter apparatus for determination of impact sensitiveness.Explosivstoffe, 14, 49-55.(b) UK Sensitiveness Collaboration Committee (1980).Explosives hazard assessment, manual of tests, SCC No. 3, Test No. "1/72.
10. Wolfson, M.G. (1983).The MRL small scale gap test for the assessment of shock sensitiveness of highexplosives (MRL Report MRL-R-896). Maribyrnong, Vic.: MaterialsResearch Laboratory.
11. Parker, R.P. (1989).Establishment of a super small-scale cookoff bomb (SSCB) test facility at"MRL(MRL Technical Report MRL-TR-89-9). Maribyrnong, Vic.: MaterialsResearch Laboratory.
12. Parker, R.P.Effect of modification of the test assembly on the results of super small-scalecookoff bomb (SSCB) tests (MRL Technical Note). To be published.
13. UK Explosives Safety Certificate No. 1124A (1970). CE.
14. Spear, R.J., Nanut, V. and Dagley, .J. (1986).RDX-Polyethylene wax formulations as potential replacements for tetryl in fuzeleads, boosters and magazines (MRL Report MRL-R-1015). Maribyrnong,Vic.: Materials Research Laboratory.
15. Spear, RJ. and Nanut, V. (1987).Mechanism of and particle size effects on shock sensitivity of heterogeneouspressed explosives: Preliminary assessment of binderless RDX in fuze trains(MRL Report MRL-R-1077). Maribyrnong, Vic.: Materials ResearchLaboratory.
16. Spear, R.J. and Nanut, V. (1987).A comparative assessment of US and UK explosives qualified as replacements fortetryl (MRL Report MRL-R-1094). Maribyrnong, Vic.: Materials ResearchLaboratory.
17. Heaps, J.M. (1972).Compatibility, efficiency and permanence of plasticizers. In,Ritchie, P.D. (Ed.) Plasticisers, stabilisers and fillers, pp. 50-83. (The PlasticsInstitute, Iliffe Books, London).
SECURITY CLASSIFICATION OF THIS PAGE UNCLASSIFIED
DOCUMENT CONTROL DATA SHEET
REPORT NO. AR NO. REPORT SECURITY CLASSIFICATIONMRL-TR-91-34 AR-006-827 Unclassified
TITEPlasticized ethylene-vinyl acetate binders for
insensitive booster compositions
AUTHOR(S) CORPORATE AUTHORI.J. Dagley, R.P. Parker Materials Research LaboratoryL. Montelli and C.N. Louey PO Box 50
Ascot Vale Victoria 3032
REPORT DATE TASK NO. SPONSORSeptember, 1991 AIR 87/156 RAAF
FILE NO. REFERENCES PAGESG6/4/8-4122 17 20
CLASSIFICATION/LIMITATION REVIEW DATE CLASSIFICATION/RELEASE AUTHORITYChief, Explosives Ordnance Division
Approved for public release
Announcement of this report is unlimited
EVA Impact sensitiveness CookoffShock sensitivity
Plasticizers have been incorporated into RDX/ethylene-vinyl acetate (EVA) compositions prepared by thesolvent slurry coating technique. The effect of plasticizers on impact sensitiveness, shock sensitivity,cookoff behaviour and integrity of pressed pellets has been examined for compositions with EVA bindersof varying vinyl acetate content. A compatible EVA/plasticizer combination gave an appreciablereduction in cookoff response and impact sensitiveness. Plasticizer migration is likely to affect the long-term stability of these compositions.